- Open Access
Which is the best method of sterilization of tumour bone for reimplantation? a biomechanical and histopathological study
© Singh et al; licensee BioMed Central Ltd. 2010
- Received: 21 June 2010
- Accepted: 10 September 2010
- Published: 10 September 2010
Sterilization and re-usage of tumour bone for reconstruction after tumour resection is now gaining popularity in the East. This recycle tumour bone needs to be sterilized in order to eradicate the tumour cells before re-implantation for limb salvage procedures. The effect of some of these treatments on the integrity and sterility of the bone after treatment has been published but there has yet been a direct comparison between the various methods of sterilization to determine the one method that gives the best tumour kill without compromising the bone's structural integrity.
This study was performed to evaluate the effect of several sterilization methods on the mechanical behavior of human cortical bone graft and histopathology evaluation of tumour bone samples after being processed with 4 different methods of sterilization. Fresh human cortical tumour bone is harvested from the diaphyseal region of the tumour bone were sterilized by autoclave (n =10); boiling (n =10); pasteurization (n =10); and irradiation (n =10). There were also 10 control specimens that did not receive any form of sterilization treatment. The biomechanical test conducted were stress to failure, modulus and strain to failure, which were determined from axial compression testing. Statistical analysis (ANOVA) was performed on these results. Significance level (α) and power (β) were set to 0.05 and 0.90, respectively.
ANOVA analysis of 'failure stress', 'modulus' and 'strain to failure' demonstrated significant differences (p < 0.05) between treated cortical bone and untreated specimens under mechanical loading.
'Stress to failure' was significantly reduced in boiled, autoclaved and irradiated cortical bone samples (p < 0.05). 'Modulus' detected significant differences in the boiled, autoclaved and pasteurization specimens compared to controls (p < 0.05). 'Strain to failure' was reduced by irradiation (p < 0.05) but not by the other three methods of treatments.
Histopathology study revealed no viable tumour cell in any of four types of treatment group compared to the untreated control group.
Sterilization of cortical bone sample by pasteurization and to a lesser extent, irradiation does not significantly alter the mechanical properties when compared with untreated samples. Mechanical properties degrade with the use of high temperature for sterilization (boiling). All methods of sterilization gave rise to 100 percent tumour kill.
- Tumour Bone
- Bone Specimen
- Bone Collagen
Osteosarcoma is the most common malignant primary bone tumour. It's a high-grade tumour derived from the mesenchymal tissue. Approximately 5 per million cases per year are diagnosed in the United States . Osteogenic sarcoma is the most common bone sarcoma and the third most common malignancy in children and adolescents. The most frequent sites of origin is the metaphyseal regions of the distal femur, proximal tibia and proximal humerus, although this tumour can practically develop in any bone [2, 3].
The treatment of Osteosarcoma consists of neo-adjuvant chemotherapy, followed by surgery and finally supplemented by adjuvant chemotherapy. The surgery can either be an amputation or limb salvage surgery. Limb salvage surgery is a type of surgery primarily performed to adequately excise tumour while preserving the particular limb. It consists of complete removal of a malignant tumour with wide margins and reconstruction of the limb with an acceptable oncologic, functional, and cosmetic result.
In limb salvage surgery for bone sarcomas, there is usually a large bone surgical defect. As most of the bone sarcomas occur in the metaphyseal portion of the bone, the resection usually involves the whole proximal or distal portion of the bone including the joint. For tumours that involve the diaphyseal portion of a bone, an intercalary resection and reconstruction can be performed that saves the joints on either side.
However, as more radical resections have been developed, the need for suitable substitutes for the resected segment has become evident. The choice of reconstruction is dependent on several factors, which include the extent of tumour, the remaining bone and soft tissue, and the patient's physical demands and expectations.
Taking in consideration the long-term viability of the reconstruction in limb salvage surgery, the use of bone appears more appealing due the potential of bone remodeling and its incorporation with host bone. Recently there has been a great interest in recycling the tumour bone itself by various methods of sterilization and reimplantation. The methods describe in the literature are boiling, autoclaving, irradiation, immerse in alcohol, pasteurization and the use of liquid nitrogen. We carried out a direct comparison between the four commonly used methods of sterilization to determine the one that gives you the best tumour kill without compromising on the structural integrity of the bone.
Materials and methods
This is a prospective in-vitro study. Samples were collected from patients diagnosed with Osteosarcoma during the limb salvage procedure. We collected samples from 10 consecutive operated cases starting from January 2009 till March 2009. All these patients underwent wide resection with endoprosthetic replacement.
Specimen for biomechanical test
Bone specimens taken from the diaphyseal region is then measured and marked using a caliper. The specimen is then cut accurately to 5 pieces each measuring 2 cm × 1 cm × 0.5 cm using an electrical saw. The cutting was carried out with water cooling to prevent any rise of temperature which may lead to irreversible thermal necrosis.
Group A will undergo autoclaving, group B boiling, Group C is the control group, group D will be treated by pasteurization and group E irradiation.
Specimens for histopathology study
Sample A was Autoclaved.
Sample B was boiled.
Sample C was used as control.
Sample D was pasteurized.
Sample E was irradiated.
Autoclave (Sample A)
The samples are placed in an autoclave compatible package. The bone specimen is autoclaved at 135 degrees Celsius for 12 to 15 minutes at a pressure of 0.2 mega Pascal (twenty nine pounds per square inch) [4, 5].
Boiling (Sample B)
Specimens are placed in sterile bottle after de-freezing and boiled at 100 deg C for 30 minutes in normal saline.
Control (Sample C)
These samples are not treated with any type of sterilization technique. The specimens are soaked in a saline dish for 20 minutes served as controls.
Pasteurization (Sample D)
Specimens placed in a sterile bottle after de-freezing and kept in preheated saline at 65 C for 30 minutes (homeothermal heater).
Irradiation (Sample E)
Testing Compression test
All specimens will be fixed with buffered formalin for histological analysis. The histological features studied include viable tumour remaining after sterilization by each of the above methods.
Fixation was carried out as soon as possible after removal of the tissues (in the case of surgical pathology).
The standard solution is 10% neutral buffered formalin. Formalin is used for all routine surgical pathology tissues when an H and E slide is to be produced.
Ethical committee approval was given for this study from the University Hospital Ethical committee.
The patients were aged between 16 to 35 years with an average age of 25 years. There were six were male and four female patients. Three patients had osteosarcoma of the distal femur and seven had osteosarcoma of the proximal tibia. All cases where in stage 2b, based on Enneking staging and all of them had been treated with adjuvant chemotherapy before the surgery. Other tumors were not included in this study.
A one-way ANOVA revealed significant differences in the treated specimens on the compression test: 'stress to failure', 'strain to failure' and 'modulus' [p < (0.05)].
The results of stress to failure, modulus and strain at failure for control and treated specimens are shown.
Stress to failure
Strain to failure
Significance levels of between treatment material property differences from Tukey post-hoc tests.
Stress to failure
Structural failure is initiated when the material is stressed to its strength limit, thus causing fracture or excessive deformations. The ultimate failure strength of the material is its maximum load-bearing capacity.
The 'elastic modulus' was calculated by a linear regression over the steepest part of the stress- strain curve before any modulus reduction occurred. The 'Modulus of Elasticity' can be used to determine stress-strain relationships in the linear-elastic portion of the stress-strain curve. The linear-elastic region is taken to be between 0 and 0.2% strain, and is defined as the region of strain in which permanent deformation occurs.
This is the main ANOVA result. The significance value comparing the groups
Sum of Squares
Stress to Failure ( MPa)
Strain To Failure (%)
Deformation of the material is the change in geometry when stress is applied. Strain or reduced deformation is the deformation change among the material field. For uniaxial loading - displacements of a specimen (for example a bar element), it is expressed as the quotient of the displacement and the length of the specimen.
Significance levels of between-treatment structural property differences from Tukey post-hoc tests.
Strain to failure
Histopathological findings of the treated and untreated groups.
To produce effective treatment of bone tumours, it is essential to eradicate all tumour tissue. Extracorporeal devitalisation and reimplantation requires both a safe margin of resection and also definite eradication of all tumour cells. In 1928, Friedgood  was the first to show that Walker rat sarcoma cells were rendered non viable after heat treatment at 44°C for 30 minutes and many studies have since shown that the thermal doses for different tumour cell lines were on the same scale (Pincus and Fischer 1931 ; Johnson 1940 ; Selawry, Goldstein and McCormick 1957 ; Auersperg 1966 ; Rivard 1984 ; Inokuchi et al 1991 ). Certain devitalisation of tumour tissue requires as an absolute minimum two minutes at 60°C or 0.5 minutes at 65°C.
There have been numerous investigations utilizing pasteurization as a method of sterilization (Campanacci and Laus 1980 ). They conclude that autoclaving as a safe method for devitalising bone tumours (Enneking and Flynn 1969 ).
Kohler et al (1986)  demonstrated that there is rapid penetration of heat into the diaphyseal bones of rabbits during autoclaving at 121°C for 20 minutes and at 131°C for two minutes, respectively, and concluded that the method can be used safely for uniform and complete sterilisation of entire specimens.
The inductive capacity of bone is destroyed to a large extent after autoclaving (Burwell 1966 ; Urist and Hernandez 1974 ; Kreicbergs and Kohler 1989 ), and its osteoinductivity is also reduced with increasing temperature and increasing duration (Bernstein et al 1993 ). An increase of temperature between 80°C and 134°C is reported to reduce healing (Knaepler et at 1992 ). It is recommend to use minimum effective autoclaving time of 15 minutes at 134°C when heating large bone specimens to devitalise tumour cells.
This study is designed to examine the effects of autoclaving, boiling, pasteurization and gamma irradiation on the compressive strength and viability of the tumour cells in the recycle tumour bone.
In a bone biomechanical studies, bending, tension, compression, and torsion strength are usually measured. We studied the compression test as the transplanted bone is usually exposed to such loads in vivo.
There are several papers reporting the effect of heat treatment itself on the bone in regard to mechanical strength changes. Köhler et al  reported in a study using the diaphyseal bone of rabbits that the strength decreased to 77% in a torsional test after being autoclaved at 121°C for 20 min. Knaepler et al  reported in his study using pig cancellous bone that the compressive strength decreased to approximately 60% after 100°C treatment, but the mechanical strength was not influenced at 60°C of heat treatment.
Using data for compressive stress to failure, modulus and strain to failure, we could demonstrate there were significant effects of the various treatment procedures on these variables.
In our study after heat treatment at 100°C and above as in autoclave and boiled group, the stress to failure strength reduction was 55% and 57% respectively in the compression testing. While after heat treatment at 60°C (pasteurization), no significant decrease in strength was observed.
These results suggest that heat treatment over 100°C results in a decrease in the bone mechanical strength, but at 60°C, the heat treatment does not affect the mechanical strength of the bone.
Autoclaved and boiled sample revealed reduction in modulus by 66% and 75% (p value less than 0.05), respectively. With the exception to the strain to failure on which there were no significant effect (p value more than 0.05).
In contrast to the pasteurization and photon irradiation results, the data suggest that high temperatures significantly alter the compressive modulus and strength of the bone.
The photon irradiation treated bones were the only sample that showed significant reduction by 62% (p value less than 0.05) in strain to failure result compared to the other treated bones, and 50% reduction in stress to failure. There was no change in the modulus.
It is known that bone collagen attributes to the bone strength, and that its properties are changed by heating. Vangsness et al  reported that collagen structure changes at temperatures higher than 80°C. While Urist et al  reported that bone collagen did not shrink with temperatures below 60°C. These reports suggest that bone collagen degenerated at 100°C heat treatment, causing a decrease in the mechanical strength, while heat-treated bone at 60°C was not affected. Moreover, the decrease in the mechanical strength of heat-treated bone at 100°C was observed in the torsional test rather than the compression test. The bone strength against compression is mainly related to the bone density , while bone strength against torsioning is likely affected by the degeneration of collagen . Therefore, apparent decrease was observed in our torsional strength testing.
The cause of this dramatic degradation in the compressive modulus and strength is most likely due to damage of the bone microstructure due to heating. Whatever the cause, these data show that heat treatments of allografts or autografts should be avoided. By autoclaving trabecular bone, the strength and stiffness of the material is reduced to half of its normal. Thus, it dramatically increases the chances of early graft failure in these cases.
Histopathology study of the sterilized specimens revealed that heat treatment at minimum of 60°C for 30 minutes is adequate to produce total tumour cell eradication.
Thermobiological research has shown that it is not necessary to heat to 100°C to cause tumour cells necrosis, but more research is needed to determine the minimum exposure time at lower temperatures which will guarantee devitalisation of tumour cells.
Hatano et al  conducted a histological study and confirmed that single radiation dose of 60 Gy was adequate for complete eradication of tumour cells in grafts.
Araki N et al, Davidson AW et al and Uyttendaele et al [27–29] reported their experience of more than 70 cases without local recurrence and metastatic disease suggests that the a single radiation dose of 50 Gy is sufficient. Higher doses have been shown to reduce the revascularization and osteoconductive capability of the graft, thereby increasing the time to union and incorporation [30–32]
Autoclaving excised bone tumours as a method of eradicating the neoplastic cells has been described but has the great disadvantage of causing a marked deterioration in the biological and biomechanical properties of the resected bone 
The effect of these methods of sterilization on its osteoconductive and osteoinductive properties of autologous tumour bone is not studied here but is currently being investigated in animal models. In our center, we are currently using pasteurization as a method of tumour sterilization.
Sterilization of cortical bone sample by pasteurization and to a lesser extent, gamma irradiation does not significantly alter the mechanical properties when compared with untreated samples. All methods of sterilization give rise to total tumour kill. Mechanical properties of the bone degrade with the use of high temperature (greater than 100 degrees) such as boiling and irradiation.
The cortical bone samples for mechanical testing were resected just adjacent to the tumour mass. On macroscopic observation, the samples taken appeared uniform, therefore we assume that the tumour involvement of the bone is homogenous. But the fact that the specimen is taken just adjacent from the tumour mass, the microscopic quality of bone is likely to be altered. This may alter the mechanical testing of the specimen.
The sample size of ten in each group has an effect on the power of the analysis contributing to the study. A larger sample size would give better representation.
The study will be better supported with an in vivo study in animals on the osteoinductive properties of this sterilized bone when re-implanted back into the study subjects.
- Landis SH, Murray T, Bolden S, Wingo PA: Cancer statistics. CA Cancer J Clin 1999, 49(1):8–31. 1 10.3322/canjclin.49.1.8View ArticleGoogle Scholar
- Marcove RC, Mike V, Hajack JV, Levin AG, Hutter RV: Osteogenic sarcoma under the age of twenty-one. A review of one hundred and forty-five operative cases. J Bone Joint Surg [Am] 1970, 52: 411–23.Google Scholar
- McKenna RJ, Schwinn CP, Soonh KY, Higinbotham N: Sarcomata of osteogenic series (osteosarcoma, fibrosarcoma, chondrosarcoma, parosteal osteosarcoma, and sarcomata arising in abnormal bone): an analysis of 552 cases. J Bone Joint Surg [Am] 1966, 48-A: 1–26.Google Scholar
- Smith PA, Ku JL, Goldstein SA, Mathews LS: A Biomechanical Study of Autoclaved Autogenous Bone. Orthop Trans 1984, 8: 495.Google Scholar
- WS Smith, Struhl S: Replantation of an autoclaved autogenous segment of bone for treatment of chondrosarcoma. Long-term follow up. J Bone Joint Surg Am 1988, 70: 70–75.Google Scholar
- Friedgood HB: On the thermal death point of sarcoma and normamononuclear cells (Walker rat tumor No. 1). Archiv f experimentelle. Zellforschung 1928, 7: 243–8.Google Scholar
- Pimcus G, Fischer A: The growth and death of tissue cultures exposed t supranormal temperatures. J Exp Med 1931, 54: 323–32. 10.1084/jem.54.3.323View ArticleGoogle Scholar
- Johnson Hi: The action of short radio waves on tissues. III: a comparison of the thermal sensitivities of transplantable tumors in vivo and in vitro. Am J Cancer 1940, 38: 533-S0.Google Scholar
- Selawry OS, Goldstein MN, McCormick T: Hyperthermia in tissue cultured cells of malignant origin. Cancer Res 1957, 17: 785–91.Google Scholar
- Auersperg N: Differential heat sensitivity of cells in tissue culture. Nature 1966, 209: 415–6. 10.1038/209415a0View ArticleGoogle Scholar
- Rivard CH: The effect of autoclaving on normal and sarcomatous bone cells and on graft incorporation. In Current concepts of diagnosis and treatment of bone and soft tissue tumors. Edited by: Uhthoff HK, Stahl E. Berlin, etc: Springer; 1984:419–25.View ArticleGoogle Scholar
- Inokuchi T, Ninomiya H, Hironaka R, Yoshida S, Araki M, Sano K: Studies on heat treatment for immediate reimplantation of resected bone. J Craniomaxillofac Surg 1991, 19: 31–9.View ArticleGoogle Scholar
- Campanacci M, Laus M: Local recurrence after amputation for osteosarcoma. J Bone Joint Surg [Br] 1980, 62-B: 201–7.Google Scholar
- Enneking WF, Flynn LM: Effects of various agents on tumor-bearing implants in bone. Clin Orthop 1969, 67: 231–42.View ArticleGoogle Scholar
- Köhler P, Kreicbergs A, Stromberg L: Physical properties of autoclaved bone. Acta Orthop Scand 1986, 57: 141–145. 10.3109/17453678609000888View ArticleGoogle Scholar
- Burwell RG: Studies in the transplantation of bone. Vifi. Treated composite homogmft-autografts of cancellous bone: an analysis of inductive mechanisms in bone transplantation. J Bone Joint Surg [Br] 1966, 48-B: 532–66.Google Scholar
- Urist MR, Hernandez A: Excitation transfer in bone. Arch Surg 1974, 109: 486–93.View ArticleGoogle Scholar
- Kreicbergs A, Kohler P: Reconstruction of large diaphyseal defects by autoclaved reimplanted bone: an experimental study in the rabbit. In Bone transplantation. Edited by: Aebi M, Regazzoni P. Berlin, etc: Springer; 1989:198–208.View ArticleGoogle Scholar
- Bernstein A, Vannini R, Ochsner P: Der Einfiuss erhOhter Temperatur auf die Osteoinduktion. Orthopadie Mitteilungen 1993, 23: 99.Google Scholar
- Knaepler H, Von Garrel T, Seipp HM, Ascherl R: Experimental studies of thermal disinfection and sterilization of allogeneic bone transplants and their effects on biological viability. Unfallchirurg 1992, 95: 477–84.Google Scholar
- Knaepler H, Haas H, Puschel HU: Biomechanische Eigenschaften thermisch und radioaktiv behandelter Spongiosa. Unfallchirung 1991, 17: 194–199. 10.1007/BF02588686View ArticleGoogle Scholar
- Vangsness CT, Mitchell W, Nimni M, Erlich M, Saadat V, Schmotzer H: Collagen shortening. Clin Orthop 1997, 337: 267–271. 10.1097/00003086-199704000-00030View ArticleGoogle Scholar
- Urist MR, Silverman BF, Buring K, Dubuc FL, Rosenberg JM: The bone induction principle. Clin Orthop 1967, 53: 243–283.View ArticleGoogle Scholar
- Carter DR, Hayes WC: Bone compressive strength. The influence of density and strain rate. Science 1976, 1174: 194–195.Google Scholar
- Peter K, Andris K, Lennart S: Physical properties of autoclaved bone. Acta Orthop Scand 1986, 57: 141–145. 10.3109/17453678609000888View ArticleGoogle Scholar
- Hatano H, Ogose A, Hotta T, Endo N, Umezu H, Morita T: Extracorporeal irradiated autogenous osteochondral graft: a histological study. J Bone Joint Surg [Br] 2005, 87-B: 1006–11.View ArticleGoogle Scholar
- Sanjay BK, Moreau PG, Younge DA: Reimplantation of autoclaved tumour bone in limb salvage surgery. Int Orthop 1997, 21: 291–297. 10.1007/s002640050171View ArticleGoogle Scholar
- Araki N, Myoui A, Kuratsu S, Hashimoto N, Inoue T, Kudawara I, Ueda T, Yoshikawa H, Masaki N, Uchida A: Intraoperative extracorporeal autogenous irradiated bone grafts in tumor surgery. Clin Orthop 1999, 368: 196–205.View ArticleGoogle Scholar
- Davidson AW, Hong A, McCarthy SW, Stalley PD: En-bloc resection, extracorporeal irradiation, and re-implantation in limb salvage for bony malignancies. J Bone Joint Surg [Br] 2005, 87-B: 851–7.View ArticleGoogle Scholar
- Currey JD, Foreman J, Laketic I, Mitchell J, Pegg DE, Relly GC: Effects of ionizing radiation on the mechanical properties of human bone. J Orthop Res 1997, 15: 111–17. 10.1002/jor.1100150116View ArticleGoogle Scholar
- Hamer AJ, Strachan JR, Black MM, Ibbotson CJ, Elson RA: Biomechanical properties of cortical allograft bone using a new method of bone strength measurement: a comparison of fresh, fresh frozen and irradiated bone. J Bone Joint Surg [Br] 1996, 78-B: 363–8.Google Scholar
- Sabo D, Brocai DR, Eble M, Wannenmacher M, Ewerbeck V: Influence of extracorporeal irradiation on the reintegration of autologous grafts of bone and joint: study in a canine model. J Bone Joint Surg [Br] 2000, 82-B: 276–82. 10.1302/0301-620X.82B2 .9447View ArticleGoogle Scholar
- Böhm P, Springfeld R, Springer H: Reimplantation of autoclaved bone segments in musculoskeletal tumor surgery: clinical experience in 9 patients followed for 1.1 - 8.4 years and review of the literature. Arch Orthop Trauma Surg 1998, 118: 57–65. 10.1007/s004020050312View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.